Abstract
Motion of growing dendrites is a common phenomenon during solidification but often neglected in numerical simulations because of the complicate underlying multiphysics. Here a phasefield model incorporating dendritemelt twophase flow is proposed for simulating the dynamically interacted process. The proposed model circumvents complexity to resolve dendritic growth, natural convection and solid motion simultaneously. Simulations are performed for single and multiple dendritic growth of an Albased alloy in a gravity environment. Computing results of an isolated dendrite settling down in the convective supersaturated melt shows that solid motion is able to overwhelm solutal convection and causes a rather different growth morphology from the stationary dendrite that considers natural convection alone. The simulated tip growth dynamics are correlated with a modified boundary layer model in the presence of melt flow, which well accounts for the variation of tip velocity with flow direction. Polycrystalline simulations reveal that the motion of dendrites accelerates the occurrence of growth impingement which causes the behaviors of multiple dendrites are distinct from that of single dendrite, including growth dynamics, morphology evolution and movement path. These polycrystalline simulations provide a primary understanding of the sedimentation of crystals and resulting chemical homogeneity in industrial ingots.
Introduction
Dendritic crystal growing from melt often undergoes a variety of physical phenomena and their interactions. One important phenomenon that has been neglected for a long term is the movement of growing crystal. In both experiments and practices, motion of crystal occurs inevitably when the melt is solidified under gravity environment^{1,2}. The motion of solid mainly stems from two forces: the gravitydriven moving force induced by density difference between the crystallizing dendrites and the melt, and external forces exerted by specific industrial processing, such as mechanical vibration, electromagnetic stirring. Solid motion is a crucial factor for microstructure formation and thereby the properties of castings. Dendrites move relative to the melt, not only altering the distribution of temperature and concentration fields, but also in turn affecting the shapes and growth dynamics^{3}. For instance, it is generally realized that the motion of equiaxed dendrites is responsible for the coneshape negative segregation in the bottom of large steel ingot^{4,5,6}.
However, despite the fact that abundant experimental, theoretical and numerical studies concerning dendrite growth under diffusion and convection have been performed during the past several decades, direct studies involving dendrite motion are rarely reported. Comprehensive understanding of its effect on dendritic growth still remains a pending issue. This is because handling the coupled dynamical behaviors between moving solid, flowing melt and growing dendrites presents a significant challenge. Experimentally, the conventional method by postmortem analysis of the sample only provides a frozen solid metallography, which is limited to confirm whether crystals moving or not during solidification, let alone the analysis of its influence on crystal morphology. Direct in situ observation is a privileged choice of studying the movement of dendrite but always limited for special materials or experimental configurations. Appolaire et al. studied the influence of movement of equiaxed dendrites on their growth kinetics using NH_{4}ClH_{2}O solution^{7,8}. The results showed that the settling of dendrite greatly promoted the growth kinetics even for weak settling velocities. Badillo et al. carried out several experiments to measure tip velocities of six primary dendrite arms of cubic SCNacetone alloy and investigated the effects of settling speed and inclination angle on growth dynamic in details^{9}. Their experimental results agree well with the boundary layer model derived from previous works^{10,11}. However, these experimental investigations are unable to clarify the coupled effect of thermosolutal convection on the dendritic growth process.
In order to exactly recover what happens in solidification simulations, the underlying multiphysics, including melt convection, solid movement, thermal and solutal diffusion, and the interplays among these effects are necessitated to be incorporated into the numerical models. DoQuang and Amberg proposed a combination of phasefield model with a fictitious domain method to simulate a settling dendrite due to gravity^{12}. The translation and rotation of a dendrite were successfully represented in the simulation. Medvedev et al. developed a combination of phasefield method with Lattice Boltzmann method (PFLB in abbreviation) to simulate mobile dendrites in a flow^{13}. Recently, Rojas et al. and Takaki et al. also used the PFLB method to simulate motion and growth of a dendrite^{14,15}. Both methods consist of two parts: the phasefield model is implemented to calculate the growth of dendrites, while the fictitious domain method or Lattice Boltzmann method is employed to compute the motion of liquid and solid. In practice, of these methods in calculating solid moving velocity, precise tracking of the solid and liquid interface is required to calculate the total force and torque acting on the solid through integrating viscous stress and pressure across the interface. Given the complex morphology of dendrite, these approaches encounter a delicate numerical treatment of the momentum exchange between solid and liquid, which is in particular intricate when simulating polycrystalline growth. Besides the overhead in keeping track of moving interfaces, these methods lose efficiency when interfaces undergo topological changes such as merging of two neighboring dendrites with a small misorientation, detaching of sidebranches and cracking of dendrite arms^{16}.
In this paper, an optional model for dendritic growth and motion is presented that permits the simulation without calculating the force acting on the solid by melt flow and handles topological changes conveniently. This is accomplished by extending the conventional phasefield model coupled with NavierStokes equations for twophase flow. Phasefield model has been validated to offer a straightforward route for conducting twophase flow simulations successfully^{17,18,19}. A wide range of twophase flow problems including Rayleigh–Taylor instability^{20}, HeleShaw flow^{21}, bubble rise and coalescence^{17}, Marangoni flow^{22} are well solved by this method. Moreover, since all the governing equations are partial differential equations which can be solved in a unified framework, significant simplification in the code structure can be achieved in respect of computation. Through comparing the calculations with several typical solidliquid twophase flow examples, the model is verified and applied to simulate motion of dendrites with melt convection in Al4wt.% Cu alloy solidification. Its effects on the dendritic growth dynamics are also illustrated and clarified.
Model Description
The phasefield model proposed by Karma for alloy solidification^{23} and the procedures by Warren et al. for polycrystalline materials^{24} are combined to simulate dendritic alloy solidification from a supersaturated liquid melt. The phasefield parameter ϕ is used to indicate the distribution of the phases, with ϕ = ±1 inside the bulk solid and liquid, respectively. Similar to previous work for solid motion^{12,13,14,15,25}, the advection term is added into the evolution equation in order to update the position of solid phases, where is the liquid flow vector. Then the phasefield equation yields to
where and W(ψ) = W_{0}a_{s}(ψ) are relaxation time and interface thickness with ψ = α_{n} − α, respectively. The symbol i stands for x and y axis, respectively, and it obeys Einstein summation convention. The anisotropy angle α_{n} is the angle between interface normal and x coordinate axis and α is crystallographic orientation. The simplified fourfold anisotropy function a_{s}(ψ) = 1 + ε cos4ψ is adopted with ε the anisotropy strength of surface energy. λ = 0.8839W_{0}/d_{0} is the coupling coefficient between phase field ϕ and dimensionless concentration field U. d_{0} = Γ/[mc_{0}(1 − k)] is chemical capillary length with m liquidus slope and k solute partition coefficient, Γ GibbsThomson coefficient, c_{0} initial concentration. The choices of τ, W, and λ, same as that of Karma^{23} lead to zero interface kinetics, hence Eq. (1) only focuses on slow solidification. The last two terms on the righthand side account for the effect of gradient of crystal orientation angle on the phase field for multiple grains. g(ϕ) = [(1 + ϕ)/2]^{2} is a monotone function in the interval [−1, 1], and h(ϕ) takes the same form as g(ϕ). And s = W_{0}/1.06 and e = W_{0}/1.875 are angle gradient coefficients that can be related to grain boundary properties^{25}. The governing equation for solute conservation is modified from the diffusionlimited model proposed by Karma^{23} to account for the convective transport of solute, i.e.
where c is solute concentration and. is a solute flux from the solid to the liquid along the direction normal to the interface to eliminate the unphysical effects induced by the finite thin interface. u is the dimensionless variable for c which is given as . The variable u measures the departure of the chemical potential from its equilibrium value for a flat interface at temperature T_{0} where the liquidus concentration is equal to c_{0}. To circumvent numerical computations of exponential and logarithm functions, a new variable U = (e^{u} −1)/(1 − k) is introduced. Replacing the concentration c in Eq. (2) with dimensionless U, the solute conservation equation is rewritten as
where D is the solute diffusivity in liquid. Here, it may be noticed that Eq. (3) has already considered the solute transport by the movement of solidified dendrites. For polycrystalline solidification, the crystallographic orientation evolution which includes crystal rotation reads^{24,25,26}
where τ_{α} = 0.1τ_{0} is a kinetic scaling factor for orientation field and P(e∇α) is an inverse mobility function, P(w) = 1 − (1 + μ/e)exp(−βw), where μ = 10^{3}W_{0} and β = 10^{5} are kinetic coefficients that respectively control the relaxation time in the bulk and grain boundary regions^{24}. The curl term on the left hand side of Eq. (4) represents the torque force induced by melt flow on the rotation of a crystal. In the model, the solid is not artificially assumed rigid but with high viscosity. This assumption refers to the schemes of conventional diffusive interface model for two incompressible viscositymatched fluids^{17,18}. The advantage of this method is that the motion of liquid and solid can be calculated simultaneously within one set of governing equations. Phasefield simulations using this model for incompressible flow of two phases of which the density ratio is close to 1000 and viscosity ratio is close to 70 demonstrate that the model is valid for flow problems with large density and viscosity ratios^{19}. This conclusion is confirmed by further simulations^{27} where the viscosity and density ratios of two phases are 100 and 1000, respectively. It can be roughly extrapolated that the phasefield model can handle twophase flow problems with large property contrast. In this work, the liquid is assumed Newtonian and incompressible while the convection is laminar. With the help of the concept of phasefield model for two liquid phases flow, the unified flow equations in the entire domain is therefore described as
where p is the pressure, is the gravity acceleration vector, α_{c} is the solutal expansion coefficient, c is the solute concentration, ρ_{s} and ρ_{l} are the solid density and liquid density, respectively. Here the way to deal with density variation is to use the classical Boussinesq approximation^{17,28}. The second term on the right hand of Eq. (5) is responsible for buoyant force in melt induced by variation of solute concentration, while the third term accounts for gravitational force due to density difference between solid and liquid. ν(ϕ) = ν_{s}(1 + ϕ)/2 + ν_{l}(1 − ϕ)/2 is a linear average of the kinematic viscosity of solid ν_{s} and liquid ν_{l}. The mass conservation equation is given as
In order to increase computational efficiency, the adaptive finite element method is adopted, where meshes can be dynamically coarsened or refined according to a local error indicator^{29}. The numerical implementation is based on the opensource finite element package AFEPack^{30}. A series of numerical tests are presented in the Supplementary Materials, including the rising of a circular particle, rotation of a growing dendrite at a constant angular velocity and single crystal in a forced shear flow. These numerical tests verify the accuracy of the proposed model in handling dendritemelt two phase flow and the choice of interface width parameter, W_{0} (see Figs S1–S5 and corresponding analysis in the Supplementary Note).
Results and Discussion
The model is then applied to simulate the dendritic solidification under gravity environment. The selected alloy system for simulations is Al4wt.% Cu, of which the physicochemical parameters as well as the applied solidification parameters are listed in Table 1. It should be noted that surface energy anisotropy strength ε_{4} is set to be 0.05 for expediency to make the dendrites grow more quickly rather than 0.0094~0.0106 obtained by experimental measurements by Liu et al.^{31}. Since the solidification velocity is slow, the phasediagram is in localequilibrium, in accordance with zero kinetic undercooling assumption in the phasefield governing equation. The dendrite grows under an isothermal (i.e. a constant supersaturation) condition. Hence parameters, including the liquidus slope and solute partition coefficient, are constants which are extracted from the phasediagram of AlCu alloy at a given undercooling.
Simulations of a dendrite settling down in a gravity environment
A free crystal growth is always of importance to single out the underlying evolution dynamics. Hence, the potential of the built model is first addressed via simulation of an equiaxed dendritic crystal growth in consideration of solutal convection and solid phase motion. This simple situation permits a clear recognition of these two effects on equiaxed crystal growth.
The simulation is conducted in a domain with size of 4000 × 7000 (856 μm × 1498 μm). Zeroflux Neumann condition is imposed on the boundaries of the computational domain for both phasefield and solute concentration equations, which is always valid in the following simulations unless otherwise stated. Noslip boundary condition is applied to all the walls of the domain for the NavierStokes equations. A round seed nucleates in the upper part of the domain to guarantee the sufficient long path for the dendrite to move downwards in a gravity environment. It may be noticed that unlike the Albased alloy with higher concentration of cooper, i.e. Al10wt.% Cu or above, the solid density for Al4wt.% Cu alloy is larger than liquid and hence dendrite settling is expected^{2}. This phenomena is convinced in the in situ and realtime observed experiment of Al4wt.% alloy^{32}, where some dendrites moved downwards slightly. Figure 1(a–c) shows the snapshots of dendritic morphology and concentration contours of the dendrite evolving with solidification time. Obviously, due to gravity effects the dendrite settles down as it grows from the saturated melt. What’s more, to keep local equilibrium, the heavier solute Cu is rejected from solid into adjacent liquid, and results into a downward flow along the solidliquid interface. This solutal convection contributes another force to the movement, pushing the dendrite settling faster. Therefore, solid sedimentation is not only caused by the gravity force induced by density variation between two phases, but also is accelerated by solutal convection. For purpose of comparison, the growth of a stationary dendrite which only considers the solutal convection effect is provided in Fig. 1(d–f). The corresponding flow field and velocity magnitude of these two cases are shown in Fig. 2. Overall, settling motion of the solid exerts a large interfacial drag force on the liquid and pulls the liquid downwards, apparently contrast to the weak flow for stationary dendrite that considers solutal convection alone. Because of the symmetry pattern of the melt flow along the vertical crystal axis, the mobile dendrite does not exhibit obvious rotation during settling. As a further validity to the twophase flow model, the velocity in the solid region appears as monolithic flow, which is shown by the isolines of magnitude in Fig. 2(b).
At the beginning of solidification for both cases, the melt flow is weak, hence, transportation of solute by convection is limited and crystal growth is controlled by diffusion. This is reflected by the symmetry shape of solute isolines around the equiaxed crystal in Fig. 1(a,d). However, as solidliquid interface progresses further into melt, the symmetry breaks down in both cases, featured by the compressed (and stretched) isolines around the vertically growing arms, as shown in Fig. 1(b,c,e,f). In the case of considering solid motion, the largest solutal gradient lies ahead of the downward growing tip, totally contrary to the situation only considering solutal convection. This is because although the rejected solute sinks down from the upper arm to the lower one, settling motion causes the tip front of the downward growing arm penetrating into the liquid, which shortens the thickness of solute boundary layer dramatically. The different solute profile surrounding the dendrite thus results in pronounced different morphology between these two cases, and here is hence evident that the motion of dendrite is capable of overwhelming the effects induced by solutal convection. However, this situation would change as Δρ_{sl}/Δρ_{c} approaches to unit with Δρ_{sl} the solidliquid density difference and Δρ_{c} the density resulting from solutal expansion. Presently, the ratio approximates to 11.
Figure 3 shows the time evolution of maximum melt flow velocity which keeps increasing for the two cases. The increment of melt flow driven by solutal convection is ascribed to more solute rejected into the melt ahead of the interface, while for the dendrite considering solid motion, the larger increase amplitude should be attributed mostly to the dendrite growing into larger size. According to the Stokes’ law, the floating or settling velocity of a particle in liquid is proportional to the square of the particle geometrical size. When the dendrite moving closer to the bottom wall of the domain, the viscosity boundary layer of convection is restricted, which hence weakens the dragging flow. Thus, the melt flow velocity reaches a peak value and then decreases at the end of simulation. After the initial rapid increase and before the decrease from the peak, the flow velocity considering solid motion keeps around 24 times of that only considering solutal convection. And the corresponding fluid Reynolds number varies from initial 0 to the end 3. Here in the calculation of Re_{L}, length of the computational domain is chosen as the characteristic length L, and the settling velocity of the dendrite is selected as the characteristic velocity V. Apparently, the type of flow is laminar, consistent with the assumption.
As is described above, when the motion of dendrite is taken into account, the flow differs a lot from that only driven by solutal buoyancy. Therefore, dendritic growth dynamics certainly varies with this alteration of flow. Detailed dendritic tip growth velocity in two cases are quantitatively compared in Fig. 4. At the early stage of solidification, the melt convection in both cases is so weak that its influence on dendrite growth is not obvious as indicated by the coincide curves. Gradually, the difference between the three tips becomes more and more noticeable. When only considering the convection driven by solutal buoyancy, the upward tip grows much faster than downward and middle tips. The growth rate of upward tip is about 1.5 times larger than that of downward tip and 1.2 times larger than that of diffusioncontrolled steadystate growth. Nevertheless, when taking account of solid motion, the growth of vertical tips presents rather different behaviors. The downward tip grows in a much higher velocity than that of upward and middle tips. Owing to continuous increase of settling speed of the dendrite, the growth rate of the downward tip increases gradually after the initial rapid decrease rather than reaches a plateau. Whereas, the growth of upward tip is heavily constrained. Because of the strong convection, the dendrite growth is controlled by flow, as denoted by the significant departure of growth rate from the diffusioncontrolled steadystate dendrite. At the end of simulation, the downward tip growth velocity is around 4.0 times higher than the diffusioncontrolled velocity.
Although the relative relation among three tip velocities in two cases seems totally opposite, the growth follows the same underlying physics, i.e. the speed strongly depends on the solute gradient and the tip undercooling. For the stationary dendrite, melt convection compresses the solute boundary layer and promotes the upstream tip growth by taking rejected solute away adequately, while it loosens the concentration isolines adjacent to the downstream arm and retards its tip growth by accumulating solute adjacent to the tip front. However, though the pattern of melt convection is similar to that of stationary dendrite, the solute gradient is steeper ahead of the downward tip for the mobile dendrite because of the fast settlement which narrows the distance between the tip interface and bulk melt. This leads to the tip interface contacting the “fresh” melt closely and thereby a high tip undercooling.
Since the solutal convection which descends along the solidliquid interface accelerates the settlement of dendrites through exerting a downward force, simulation of mobile dendrite free from solutal convection is performed to clarify this effect on settlement for convenience. The instantaneous settling velocities of mobile dendrite with and without consideration of solutal convection are plotted in Fig. 5. Overall, the settling velocity increases in a linear fashion with time for both cases whose evolution feature is in the same manner as the result obtained by Badillo et al.^{9}. When solutal convection is taken into consideration, the dendrite settles much faster. For the present simulation configuration, the settling velocity increases up to 20% at the late solidification stage. Hence, it demonstrates that the interaction between solutal convection and solid motion is in a coupled behavior. When convective flow is in line with the moving direction of solid, both convection and movement will be strengthened, while in an opposite direction, their dynamics will be weakened. This phenomenon is further evidenced and analyzed in the following simulation of polycrystalline condition.
Correlating the simulations with an analytical theory
The influence of dendrite settlement on growth dynamics of transparent alloy has been studied experimentally by Badillo et al.^{9}. Based on the experimental data, the boundary layer model which accounts for the effects of thermosolutal convection on free dendritic growth of alloys^{10,11,33,34} is modified to address the flow angle dependence. The modified model is found to predict well the variation in the tip velocity due to crystal rotation and settling speed change^{9}. Here the phasefield simulation of single mobile dendrite is examined by the solution of the analytical model. It should be noted that the 3D Ivantsov paraboloid solution rather than the 2D parabolic equation is adopted in the analytical model here. According to the study by McFadden and Browne^{35}, dendrite tip growth rate calculated by 3D Ivantsov solution can be more than 10 times larger than that by 2D results at slightly high undercooling. However, the numerical results by phasefield model for the tip velocity are different for 3D versus 2D by a factor of only 1.76~2.0^{36,37}. The mismatch ratio between phasefield simulation and analytical solution leads to the comparison intricacy. As the 3D analytical solution predicts better the experimental data, hence the modified 3D Ivantsov function that considers flow effects is utilized to compare with phasefield simulation. The boundary layer model in presence of convection is deduced based on the framework of LGK model for diffusioncontrolled free dendrite growth^{38}. As the temperature is assumed uniform in the system and the undercooling is low, the effects of latent heat and interface attachment kinetics are neglected. The total undercooling is composed of
where ΔT_{c}, ΔT_{r} are solutal and curvature undercooling, respectively. And R is dendrite tip radius, P_{c} is solutal Péclet number, P_{c} = RV/2D_{l}, where V is dendrite growth velocity. I_{V}(P_{c}) is Ivantsov function of P_{c} and I_{V}(P_{c}) = P_{c}exp(P_{c})E_{1}(P_{c}) with E_{1} the exponential integral function. The tip radius, R, is given by
It is assumed that the selection parameter σ^{*} is not influenced by convection (here σ^{*} = 1/4π^{2}) in the boundary layer model. In presence of flow, the classical Ivantsov solution for solutal saturation, Ω_{C}, is replaced with the following modified stagnant film solution
where , in which c^{*} is solute concentration in the liquid at solidliquid interface and δ_{c} is solutal boundary layer thickness^{11}
where Re is Reynolds number, , in which V_{s} is the instantaneous settling velocity, Sc is the Schmidt number, , a = 0.5773, b = 0.6596, c = 0.5249. f(θ) is an angular factor accounting for the effect of growth directions with respect to gravity on the dendrite tips, and θ is the socalled Eulerian angle defined in the same way by Badillo^{9}: θ = 0° for downward growing tip, θ = 90° for perpendicular ones, and θ = 180° for upward growing one. Apparently, Eq. (9) resumes to Ivantsov relations when the boundary layer thickness is infinitely large or f(θ) is vanished. The exact form of f(θ) adopted by Sekerka et al.^{11,34} is
As noted by Badillo et al.^{9}, the value of f(θ) is not negative and it would always result in a greater tip velocity in presence of convection than the diffusion value. To circumvent this irrationality, they fitted the experimental data and obtained a fifth order polynomial^{9}. Obviously, the complicate polynomial formulation of f(θ) is not theoretically rigorous, hence a simpler expression derived from Eq. (11) is proposed
where K_{1} is an amplitude parameter controlling the effect of Eulerian angle on the growth dynamics and K_{2} is an asymmetry factor, when it is set to 0, it implies that the calculated velocity at θ = 90° will have the same value to the diffusional occasion. The original data points of f(θ) extracted from phasefield simulation at t = 0.51 s when the perpendicular arm growth reaches steady state are shown in Fig. 6, in cases of three different initial orientations (0°, 20°, 60°). The leastsquares fitting is adopted to find the optimal values of K_{1} and K_{2}, which are then convinced to be 0.87 and 0.22, respectively, just as the solid line in Fig. 6 illustrates. Plotting of the polynomial^{9} is also imposed in the figure. As expected, the phasefield simulated data deviate a lot from the polynomial curve, in particular at the angle between 20° and 70° where the polynomial curve is almost flattened, physically not reasonable. Figure 7 shows the comparison of the calculated tip velocities versus settling velocities between phasefield simulations and the analytical model. The comparison begins when the tip growth of perpendicular arm arrives at steady state. Generally, with the proposed f(θ) of Eq. (12) the analytical predictions shows a good agreement with phasefield simulation, especially at lower settling velocity. The underestimation of growth velocity for the downward growing arm at higher settling velocities may be mainly due to sharply changes of the solute boundary layer ahead of the tip when the dendrite moves very fast.
Polycrystalline growth in gravity environment
The dendritic motion and melt convection during polycrystalline solidification will differ dramatically from that of single crystal growth. The interaction between crystal growth, solutal convection and solid motion becomes more complex because of the impinging effect of multiple dendrites. This results from that when two crystals get close, both the symmetry of solutal boundary and flow pattern which are observed during single free dendrite growth are destroyed. As well to clarify such interacting mechanism during polycrystalline growth, simulations with solutal convection alone and considering both solid and liquid flow are performed as shown in Figs 8 and 9. In simulations, 12 nucleation seeds are randomly placed initially with random orientations in a domain with size of 642 μm × 642 μm. For the simulation considering motion of dendrites, initially, similar to the single crystal growth, all crystals move downwards and a descending melt flow generates around each one, being absence from interactions with others, as shown in Fig. 9(a). As a result, dendrites settle vertically. As crystals growing into larger size, the surrounding flow comes to interact with others. Consequently, the initial symmetric flow vortexes deform and merge with others, inducing strong interdendritic convection, just as illustrated in Fig. 9(b,c). This convergence interrupts the original vertical downward flow, and then imposes an inclined force to the dendrites. Ultimately, at the end of simulation, crystals accumulate at the bottom of the domain, forming a sedimentation zone as described in Fig. 9(d). It may be noticed that during settling of these dendrites, rotational movement is not apparent which can be ascribed to the not sufficient shear force that acts upon the dendrites by the melt flow. When compared with growth of dendrites in Fig. 8, generally, there is no obvious difference of the flow pattern in liquid that can be observed for the two cases at early stage but the lower flow strength in simulation driven by solute buoyancy alone. Interestingly, the ratio of maximum flow velocity between the two cases is around the value of Δρ_{sl}/Δρ_{c}.
The sedimentation zone constantly occurs in experiments. Beckermann and Wang performed experiments to study the equiaxed dendritic solidification of NH_{4}ClH_{2}O solution in a square cavity^{39}. It was observed that the crystals settled down during solidification and gradually formed a sedimentation bed on the cavity floor, which was a zone of negative segregation. This phenomenon is further confirmed and characterized through more delicate experiments^{40,41}. Both present simulation and these experiments have demonstrated that the motion of crystals due to gravity is common and plays a crucial role on the formation of the macrosegregation pattern. Nevertheless, since the solute is also heavier than the solvent in present case, it also tends to accumulate at the bottom of domain, as indicated by the solute contour in Fig. 9(d). In this situation, the negative segregation resulting from the sedimentation will be reduced to some extent. Also as demonstrated by Wang et al.^{2} with the liquid concentration increasing due to solute rejection, the density difference between solid and liquid reduces which would further lighten the macrosegregation. On the contrary, for other alloy systems, such as FeC alloy, the lighter rejected solute C floats upwards, while the solidified crystals that are lack of C settle down. In this situation, the negative segregation will be quite severe.
In order to clearly demonstrate the motion of solid during polycrystalline solidification, the walking routes of two selected dendrites, No. 4 and 9 as marked in Fig. 9(c), are tracked in Fig. 10. Changes of centroid locations of the two dendrites are recorded relative to their initial positions. From the trajectory, it is clearly observed that No. 4 dendrite firstly tilts to right during its settling, then moves back to left. In contrast, No. 9 dendrite keeps the tendency of tilting to right, and settles down slowly in the vertical direction. These different behaviors of two dendrites are due to their exposure to different flow environments as illustrated by the flow field in Fig. 9. The measured settling velocities of these two dendrites, together with the isolated mobile dendrite in Fig. 1 are plotted in Fig. 11. It can be seen that unlike the linear acceleration of the isolated dendrite, the two dendrites experience an alternation from acceleration to deceleration, and both their absolute velocities are much lower than that of isolated one. This phenomenon demonstrates that during polycrystalline growth, the flow is able to give a lifting force which counteracts the gravity to a dendrite. At the end of simulation, i.e. after 1.1 s, the velocities of the two dendrites tends to 0 due to their arrival at the sedimentation zone. Apparently, dendrites during polycrystalline solidification experience different drag and buoyant forces and thus the overall flow and motion behavior are rather distinct from those of the single dendrite^{42}. The walking routes of multiple dendrites as well show obvious sensitivity to the melt flow though the motion depends on the density difference between solid and liquid. These motion behaviors therefore interpret the applied external field (e.g. electromagnetic field) to control microstructure of castings via generating external forces on the solidifying crystals to overwhelm the gravity.
The convection and solute distribution around a dendrite during polycrystalline solidification is quite different from that of free isolated dendrite. This is because of the interactions between dendrites, such as the softimpingement stemmed from the overlapped solute boundary layers^{32,43}. Dendrites in polycrystalline material usually have random orientations, which results in the uncertainty of the interplay and their growth dynamics. For quantitative illustration of these complexities, the growth velocities of twelve dendrites versus the Eulerian angle are measured in Fig. 12. Conclusions can be drawn from these results as follows. (1) At t = 0.21 s, not only arm tips at different directions of one dendrite but also dendrites with different orientations show almost the same growth velocity, approximate to 75 μm/s. This is the typical characteristic of free dendrite growth at the initial stage^{32,43}, i.e. growth velocities are mainly controlled by diffusion, seldom affected by convection and softimpingement effects. (2) At t = 0.64 s, the solid motion effect dominates the growth. It can be seen that the velocities satisfy the outcome obtained in the above section for single dendrite, i.e., the larger the Eulerian angle is, the more slowly the arm grows. The velocity varies from 15 μm/s to 80 μm/s. (3) At the end of simulation t = 1.17 s, the dominant effect switches to softimpingement effect, since the dendrites at this time almost settle down to the bottom of the domain, and accumulate together to form the deposition zone. The solute piles up heavily between dendrites, which decreases or even eliminates the tip undercooling. In this situation, most dendrites growing slowly and some of them behave against to the convection effect. For instance, the upward growing arm of No. 1 dendrite exhibits a larger velocity than the downward arm.
However, although the simulations have taken into consideration the effects of solutal convection and solid motion, one interesting phenomenon that the variation of solid fraction with time does not show much visible difference from that of cases under the diffusioncontrolled or just considering the solutal convection alone. The simulated dendritic morphologies under pure diffusion can be seen in the Supplementary Materials (Fig. S4). The evolution of solid fraction is shown in Fig. 13(a), and the difference between mobile dendrites and stationary ones with purediffusion is plotted in Fig. 13(b). Before t = 1.0 s the increment of solid fraction is free from the influence of dendrite motion and solutal convection. Afterwards, the deviation becomes noticeable, appearing as a sharp decrease of the solid fraction of mobile dendrites because of the accumulation of dendrites. This implies that the movement of dendrites accelerates the impinging process which prevents solid from growing further into melt.
Conclusion
A phasefield model for simulating dendritemelt twophase flow during binary alloy solidification is proposed. It aims to uncover the coupling phenomena between melt convection, solid motion, solute diffusion and crystal growth during solidification. Compared to previously used phasefield Lattice Boltzmann method, it is not necessary to track explicitly the interfaces between different phases or different grains to resolve the motion of crystals, but still able to predict the rotational and translational motion of a solid with complex morphology in the proposed method. Simulations of a single dendrite settling down under gravity demonstrate that the motion of solid exerts crucial effects on the dendritic growth morphology. The solid motion promotes the downstream arm growth rather than the upstream arm, which is contrary to the case under only melt convection. With the simulations of single dendritic growth at different orientations and previous experimental data^{9}, the analytical boundary layer model that predicts the effects flow on dendritic growth dynamics is modified to well relate the dendritic tip velocities with respect to flow directions. A generally good agreement is achieved between phasefield simulation considering dendrite motion and the analytical solution. The proposed phasefield model incorporating twophase flow is then extended to tackle the complex solidification phenomenon of multiple crystals. Because of dendrites motion, a sedimentation zone of crystals is observed in the simulation, which reveals the fundamental process of such phenomenon often occurred in industrial ingots. The growth dynamics, movement path and solid fraction of polycrystalline solidification are characterized in detail which uncovers the interacting process between solid motion, melt flow and crystals growth. These interactions closely relate to the stochastic factors existing in solidification, such as the amount of seeds, relative position of nucleating sites and crystallographic orientations. And hence the growth and movement of each dendrite not only depends on its own buoyant force and local solute boundary layer, but also associates to the longrange melt flow.
The extension of the model to three dimension is direct since all the coupled physical models have already been well developed separately in 3D. The simulations presented in this work are for melt flow with small Reynolds number, numerical analysis and benchmark simulations are necessitated to verify the possibility in coping with solid particle moving and rotating at high speed or flow with large Reynolds number. In addition, direct collision of dendrites in this model is neglected. The parameters in the polycrystalline phasefield model are given artificially and not derived from material properties, which makes the polycrystalline growth can not be closely related to real materials and compared with in situ experiments quantitatively^{32,43}. This deficiency may be solved using the front tracking method to calculate the orientation proposed in the ref. 44 when the grain boundary energy and rotation change of crystal orientation are included into their model.
Additional Information
How to cite this article: Qi, X. B. et al. Modeling of coupled motion and growth interaction of equiaxed dendritic crystals in a binary alloy during solidification. Sci. Rep. 7, 45770; doi: 10.1038/srep45770 (2017).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
References
Wang, C. Y. & Beckermann, C. Equiaxed dendritic solidification with convection: Part I. Multiscale/multiphase modeling. Metall. Mater. Trans. A 27, 2754–2764 (1996).
Wang, C. Y. & Beckermann, C. Equiaxed dendritic solidification with convection: Part II. Numerical simulations for an Al4 Wt pct Cu alloy. Metall. Mater. Trans. A 27, 2765–2783 (1996).
Lesoult, G. Macrosegregation in steel strands and ingots: Characterisation, formation and consequences. Mater. Sci. Eng. A 413–414, 19–29 (2005).
Olsson, A., West, R. & Fredriksson, H. Macrosegregation in ingots. Scand. J. Metall. 15, 104–112 (1986).
Wu, M. & Ludwig, A. Modeling equiaxed solidification with melt convection and grain sedimentation—II. Model verification. Acta Mater. 57, 5632–5644 (2009).
Liu, B., Xu, Q., Jing, T., Shen, H. & Han, Z. Advances in multiscale modeling of solidification and casting processes. JOM 63, 19–25 (2011).
Appolaire, B., Albert, V., Combeau, H. & Lesoult, G. Free growth of equiaxed crystals settling in undercooled NH4ClH2O melts. Acta Mater. 46, 5851–5862 (1998).
Appolaire, B. et al. Experimental study of free growth of equiaxed NH4Cl crystals settling in undercooled NH4ClH2O melts. ISIJ Int. 39, 263–270 (1999).
Badillo, A., Ceynar, D. & Beckermann, C. Growth of equiaxed dendritic crystals settling in an undercooled melt, Part 1: Tip kinetics. J. Cryst. Growth 309, 197–215 (2007).
Cantor, B. & Vogel, A. Dendritic solidification and fluid flow. J. Cryst. Growth 41, 109–123 (1977).
Gandin, C. A., Guillemot, G., Appolaire, B. & Niane, N. T. Boundary layer correlation for dendrite tip growth with fluid flow. Mater. Sci. Eng. A 342, 44–50 (2003).
DoQuang, M. & Amberg, G. Simulation of free dendritic crystal growth in a gravity environment. J. Comput. Phys. 227, 1772–1789 (2008).
Medvedev, D., Varnik, F. & Steinbach, I. Simulating mobile dendrites in a flow. Procedia Comput. Sci. 18, 2512–2520 (2013).
Rojas, R., Takaki, T. & Ohno, M. A phasefieldlattice Boltzmann method for modeling motion and growth of a dendrite for binary alloy solidification in the presence of melt convection. J. Comput. Phys. 298, 29–40 (2015).
Takaki, T., Rojas, R., Ohno, M., Shimokawabe, T. & Aoki, T. GPU phasefield lattice Boltzmann simulations of growth and motion of a binary alloy dendrite. IOP Conf. Ser.: Mater. Sci. Eng. 84, 012066 (2015).
Feng, J. J., Liu, C., Shen, R. & Yue, P. T. In Modeling of Soft Matter Vol. 141 (eds M. C. T. Calderer & A. Seheel ) 1–26 (Springer, 2005).
Liu, C. & Shen, J. A phase field model for the mixture of two incompressible fluids and its approximation by a Fourierspectral method. Physica D 179, 211–228 (2003).
Yue, P., Feng, J. J., Liu, C. & Shen, J. A diffuseinterface method for simulating twophase flows of complex fluids. J. Fluid Mech. 515, 293–317 (2004).
Shen, J. & Yang, X. A phasefield model and its numerical approximation for twophase incompressible flows with different densities and viscosities. SIAM J. Sci. Comput. 32, 1159–1179 (2010).
Jacqmin, D. Calculation of twophase Navier–Stokes flows using phasefield modeling. J. Comput. Phys. 155, 96–127 (1999).
Folch, R., Casademunt, J., HernándezMachado, A. & RamírezPiscina, L. Phasefield model for HeleShaw flows with arbitrary viscosity contrast. I. Theoretical approach. Phys. Rev. E 60, 1724–1733 (1999).
Yue, P., Feng, J. J., Liu, C. & Shen, J. Interfacial forces and Marangoni flow on a nematic drop retracting in an isotropic fluid. J. Colloid Interface Sci. 290, 281–288 (2005).
Karma, A. Phasefield formulation for quantitative modeling of alloy solidification. Phys. Rev. Lett. 87, 115701 (2001).
Warren, J. A., Kobayashi, R., Lobkovsky, A. E. & Craig Carter, W. Extending phase field models of solidification to polycrystalline materials. Acta Mater. 51, 6035–6058 (2003).
Yamaguchi, M. & Beckermann, C. Simulation of solid deformation during solidification: Compression of a single dendrite. Acta Mater. 61, 4053–4065 (2013).
Yamaguchi, M. & Beckermann, C. Simulation of solid deformation during solidification: Shearing and compression of polycrystalline structures. Acta Mater. 61, 2268–2280 (2013).
Ding, H., Spelt, P. D. M. & Shu, C. Diffuse interface model for incompressible twophase flows with large density ratios. J. Comput. Phys. 226, 2078–2095 (2007).
Lee, H. & Kim, J. A comparison study of the Boussinesq and the variable density models on buoyancydriven flows. J. Eng. Math. 75, 15–27 (2012).
Li, R. On multimesh Hadaptive methods. J. Sci. Comput. 24, 321–341 (2005).
Wang, H., Li, R. & Tang, T. Efficient computation of dendritic growth with radaptive finite element methods. J. Comput. Phys. 227, 5984–6000 (2008).
Liu, S., Napolitano, R. E. & Trivedi, R. Measurement of anisotropy of crystalmelt interfacial energy for a binary Al–Cu alloy. Acta Mater. 49, 4271–4276 (2001).
Chen, Y. et al. Quantitative phasefield simulation of dendritic equiaxed growth and comparison with in situ observation on Al4 wt.% Cu alloy by means of synchrotron Xray radiography. ISIJ Int. 54, 445–451 (2014).
Li, Q. & Beckermann, C. Modeling of free dendritic growth of succinonitrile–acetone alloys with thermosolutal melt convection. J. Cryst. Growth 236, 482–498 (2002).
Sekerka, R. F., Coriell, S. R. & McFadden, G. B. Stagnant film model of the effect of natural convection on the dendrite operating state. J. Cryst. Growth 154, 370–376 (1995).
McFadden, S. & Browne, D. J. A generalised version of an Ivantsovbased dendrite growth model incorporating a facility for solute measurement ahead of the tip. Comput. Mater. Sci. 55, 245–254 (2012).
Altundas, Y. & Caginalp, G. Computations of dendrites in 3D and comparison with microgravity experiments. J. Stat. Phys. 110, 1055–1067 (2003).
Altundas, Y. & Caginalp, G. Velocity selection in 3D dendrites: Phase field computations and microgravity experiments. Nonlinear Analysis: Theory, Methods & Applications 62, 467–481 (2005).
Lipton, J., Glicksman, M. E. & Kurz, W. Dendritic growth into undercooled alloy metals. Mater. Sci. Eng. 65, 57–63 (1984).
Beckermann, C. & Wang, C. Y. Equiaxed dendritic solidification with convection: Part III. Comparisons with NH4ClH2O experiments. Metall. Mater. Trans. A 27, 2784–2795 (1996).
Kharicha, A., StefanKharicha, M., Ludwig, A. & Wu, M. Simultaneous observation of melt flow and motion of equiaxed crystals during solidification using a dual phase particle image velocimetry technique. Part I: Stage characterization of melt flow and equiaxed crystal motion. Metall. Mater. Trans. A 44, 650–660 (2013).
Kharicha, A., StefanKharicha, M., Ludwig, A. & Wu, M. Simultaneous observation of melt flow and motion of equiaxed crystals during solidification using a dual phase particle image velocimetry technique. Part II: relative velocities. Metall. Mater. Trans. A 44, 661–668 (2013).
Karagadde, S., Bhattacharya, A., Tomar, G. & Dutta, P. A coupled VOF–IBM–enthalpy approach for modeling motion and growth of equiaxed dendrites in a solidifying melt. J. Comput. Phys. 231, 3987–4000 (2012).
Bogno, A., NguyenThi, H., Reinhart, G., Billia, B. & Baruchel, J. Growth and interaction of dendritic equiaxed grains: In situ characterization by synchrotron Xray radiography. Acta Mater. 61, 1303–1315 (2013).
Chen, Y., Qi, X. B., Li, D. Z., Kang, X. H. & Xiao, N. M. A quantitative phasefield model combining with fronttracking method for polycrystalline solidification of alloys. Comput. Mater. Sci. 104, 155–161 (2015).
Chen, Y. et al. Tipsplitting instability and transition to seaweed growth during alloy solidification in anisotropically preferred growth direction. Acta Mater. 66, 219–231 (2014).
Acknowledgements
This work is supported by the National Natural Science Foundation for Young Scientists of China (Grant No. 51401223) and the National Natural Science Foundation of China (Grant No. 51271184, U1508215).
Author information
Authors and Affiliations
Contributions
Y.C. conceived and supervised the project. X.B.Q. wrote the codes of phasefield simulations and the main manuscript text. X.H.K. and D.Z.L. provided advices on the dendritic growth dynamics in polycrystalline simulation. T.Z.G. provided advices on the simulations. All authors reviewed the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Qi, X., Chen, Y., Kang, X. et al. Modeling of coupled motion and growth interaction of equiaxed dendritic crystals in a binary alloy during solidification. Sci Rep 7, 45770 (2017). https://doi.org/10.1038/srep45770
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/srep45770
This article is cited by

Modeling of Grain Refinement and Nucleation Behavior of Mg4Y0.5Zr (wt.%) Alloy via Cellular Automaton Model
International Journal of Metalcasting (2022)

A phasefield study of the solidification process coupled with deformation
Journal of Materials Science (2021)

Heat transfer during diffusioncontrolled unidirectional solidification of binary mixtures: effect of material advection
Sādhanā (2021)

Simulations of Multiple Grains Growth of Mg–Al Alloy Semisolid Structure by PhaseFieldLattice Boltzmann Simulation
Metallurgical and Materials Transactions B (2021)

PFLBM Modelling of Dendritic Growth and Motion in an Undercooled Melt of FeC Binary Alloy
Metallurgical and Materials Transactions B (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.